2 Best Practices for Jointed Concrete Pavements / Blended Aggregates for Concrete Mixture Optimization
• Increased shrinkage, which can result in cracking • Higher permeability leading to critical saturation of the paste fraction (i.e., lower resistance to freeze-thaw deterioration) • Higher heat of hydration • Increased cost Portland cement concrete mixtures used for slipformed pavements should be designed to meet all performance objectives (strength, durability, thickness, smoothness, etc.) and delivered with a workability that produces a nearly vertical edge and minimizes the need for excessive vibration and/or hand finishing (Figure 1). A well graded aggregate system is one tool that can be used to help achieve this aim. Reducing the paste content of a concrete paving mixture (within limits) through careful management of the aggregate system is therefore desirable for improved performance and at the same time for improved sustainability. BACKGROUND Until the 1990s, the gradation of the total aggregate system was rarely considered. However, efforts by Shilstone (1990) led to development of the workability factor chart (Figure 2) among other tools. This empirical work was based on field experimentation with a focus on reducing segregation in mixtures.
The horizontal axis of the workability factor chart is the so-called coarseness factor, which is the mass of the coarse sized (>3/8 in.) aggregate divided by the sum of the masses of the coarse and intermediate (>#8 and <3/8 in.) sizes. A coarseness factor of 100 describes a grading with no intermediate aggregate, and such a mixture may be considered gap-graded. A value of 0 describes a mixture with no coarse aggregate. The vertical axis is the “workability factor,” which is the percent of the combined aggregate that passes the 2.36-mm (#8) sieve plus an adjustment for the amount of cementitious material in a mixture. The chart is divided into several zones with Zone II reported as that desirable for 3/4 in. to 2 in. aggregate nominal maximum sizes in paving mixtures. Experience has shown that staying within the Zone II box may improve the probability that a workable mixture is achieved; however, it is still possible to produce concrete with poor characteristics inside the box, and good performance is still possible outside the box. Data by Ley has indicated poor correlation between workability and information provided by this chart. A second tool is to compare the combined gradation on a cumulative passing plot in which the horizontal axis is raised to the power of 0.45. This is based on numerical modeling indicating that maximum density of aggregates is achieved when the plotted combined gradation falls on the line (Kennedy et al. 1994) (Figure 3). It has been reported that some variation off the ideal line is indeed desirable because too dense a system becomes unworkable. The third tool used to date has been the Haystack (percent retained) chart in which the amount of material retained on any given sieve was kept within the range of 8 to 18%. All three of these tools provide slightly different information. Experience has shown that none of these approaches is ideal.
Figure 2. Shilstone workability factor chart
Recent work by Ley has reported that an approach based on the Haystack chart seems to provide promise of achieving reliably workable mixtures. The work was based on re-sieving a given set of materials to adjust the amount retained on one sieve size, by increments, and then to assess the workability of a mixture with fixed proportions (Ley and Cook 2014). Workability was measured using the Box Test (Ley et al. 2012). The Tarantula curve (Figure 4) provides an envelope in which a desirable amount of material retained on each sieve is reported. The curve varies from the Haystack in that for most fractions, the upper and lower bounds are broadened, except for those on the #8 and #16 sieves that are reduced.
Figure 3. Power 45 gradation curve